Effect of morphologies and compositions of silver-based multicomponent heterogeneous nanocrystals on the reduction of 4-nitrophenol

Silver-based nanocrystals have excellent catalytic performance in various reactions, such as the reduction of 4-nitrophenol. The catalytic performance of nanocrystals varies with several parameters, including nanocrystal morphology, composition, and plasmon-induced hot electrons around nanocrystals. Here, highly heterogeneous nanocrystals (Au–Ag and Ag2S–Ag nanocrystals) fabricated on polymer films via a seed-mediated method are used as catalysts for the reduction of 4-nitrophenol, and the effect of the morphology and composition of nanocrystals on the catalytic performance is investigated. These nanocrystals on polymer films exhibit higher reusability (low catalyst loss) in catalytic applications compared to catalysts dispersed freely in the reaction solution. The excellent catalyst performance of these heterogeneous nanocrystals is attributed to their high surface area/volume ratio (flower-like nanocrystals) and strong synergistic effect (cage-like nanocrystals). These nanocrystals with special morphologies and composites showed higher catalytic performance (higher reactivity at lower catalyst contents) than silver-based nanocrystals reported in the literature. Due to the excellent plasmonic properties of Ag nanocrystals, the catalytic performance of these nanocrystals can be further enhanced by generating hot electrons around the nanocrystals under irradiation. These results demonstrated that by carefully controlling the morphology and composition of nanocrystals, it is possible to design and fabricate excellent catalysts for various reactions.


Introduction
2][3][4] One of the most common difficult-to-treat water pollutants and environmentally harmful materials was 4-nitrophenol (4-NP), which had been demonstrated to be highly toxic and carcinogenic.Interestingly, the reduction product of 4-NP, 4 aminophenol (4-AP), is a valuable material due to its low toxicity and various useful applications, such as corrosion inhibition, anticorrosion lubrication, drying agent, photographic development, etc. [5][6][7] To covert trace amounts of 4-NP in water to valuable 4-AP, cost-effective, stable, and highly active catalysts for 4-NP reduction were highly desirable.][10][11][12][13][14][15][16][17] The advantages of Ag nanocrystals as catalysts were: (1) catalytic activity can be tuned by controlling their size and shape; (2) the reaction temperature requirement was low; 9][20] Even though Ag nanocrystals were ideal catalysts for 4-NP reduction, Ag nanocrystals used as catalysts still had several issues such as easy aggregation and lower catalytic activity, which needed to be treated to improve their catalytic performance.The aggregation problem can be effectively reduced by incorporating Ag nanocrystals into substrates, such as polymer matrices. 21The lower catalytic activity can be improved by using (1) anisotropic Ag nanocrystals, such as Ag nanocubes (AgNCs), and (2) bimetallic Ag nanocrystals to replace the monometallic Ag nanocrystals. 9,15ecently, our group fabricated highly heterogenous bicomponent nanocrystals on AgNCs embedded in a polymer matrix as templates.Here, a hydrophobic layer, such as a polystyrene lm, can act as an interface to suppress the formation of bicomponent nanocrystals in aqueous solution, leading to the formation of highly heterogeneous nanocrystals with controllable morphologies and components of nanocrystals.These highly heterogeneous bicomponent nanocrystals synthesized on the hydrophobic layer also showed that these nanocrystals can be well dispersed on a polymer matrix and can also be used to address the problems of aggregation 21 and low activity as catalysts for the 4-NP reduction reaction, resulting in excellent Nanoscale Advances PAPER catalytic performance.The hydrophobic layer can also prevent the adsorption of 4-NP molecules in the matrix from affecting the evaluation of the reduction reaction and prevent the loss of heterogeneous nanocrystals during the recycling process aer the reduction reaction of 4-NP molecules in aqueous solution.
To systematically study the catalytic performance of these silverbased bicomponent nanocrystals as 4-NP reduction catalysts, several parameters were used to characterize the catalytic performance, as listed below: (1) reusability tests by comparing catalysts that were freely dispersed in the reaction solution or xed on a polymer matrix; (2) the catalyst concentrationdependent reaction rate of 4-NP reduction; (3) the catalyst shape-dependent reaction rate of 4-NP reduction (involving the effects of the surface area/volume ratio, synergetic effect, and competitive reactions); (4) the catalyst component-dependent reaction rate of 4-NP reduction; (5) the plasmon-enhancement effect (as shown in Fig. 1).
The results showed that the reusability of silver-based nanocrystals xed on a polymer matrix as catalysts was higher than that of catalysts freely dispersed in the reaction solution.Compared with the pristine AgNCs xed in a polymer matrix, the ower-like Au-AgNC and cage-like Au-AgNC nanocrystals xed in a polymer matrix had higher 4-NP reduction reactivity, which can be attributed to the high surface area/volume ratio and strong synergetic effect, respectively.However, compared with the pristine AgNC xed in a polymer matrix, the core-shell Ag 2 S-AgNC nanocrystals xed in a polymer matrix exhibited lower 4-NP reduction reactivity and reshaped nanocrystals, which may be caused by the reduction of Ag ions on Ag 2 S to Ag atoms, a competitive reaction of 4-NP reduction.Due to the excellent plasmonic properties of Au-AgNC nanocrystals, Au-AgNC nanocrystals can generate many "hot electrons" around them under irradiation in plasmonic mode.These hot electrons can be used to accelerate the reaction rate of the 4-NP reduction.Compared with the reduction of 4NP without irradiation assistance, the reduction rate of 4-NP exhibited an enhancement factor of about 1.1-1.25 times under irradiation assistance, and the enhancement factor increased with the number of hot electrons (the number of catalysts).These results provided a comprehensive understanding of the possible factors that lead to changes in the reduction reactivity of 4-NP when Ag-based heterogeneous nanocrystals were used as catalysts.This information paved the way for designing excellent catalysts for the 4-NP reduction reaction.

Results and discussion
To systematically study the catalytic performance of silver-based nanocrystals as 4-NP reduction catalysts, silver-based bicomponent nanocrystals with different morphologies, and compositions (ower-like Au-AgNCs, cage-like Au-AgNCs, and coreshell Ag 2 S-AgNC nanocrystals) were used as catalysts for NaBH 4 -assisted reduction of 4-NP in aqueous solution.Since the catalytic performance was affected by several parameters, the results were divided into several subsections with different variables to discuss the inuence on the catalytic performance: (A) reusability of catalytic performance: catalysts were freely suspended or xed on the polymer matrix; (B) the amount of catalyst used; (C) shape of bicomponent nanocrystals: owerlike Au-Ag nanocrystals (higher surface area/volume ratio) or  The rst problem with solid catalysts for water pollutant treatment was reusability: the washing step in the reused process led to a decrease in the amount of solid catalyst, which reduced the catalytic performance.Our group synthesized silver-based bicomponent nanocrystals on a template substrate, consisting of an AgNC array partially embedded in a polymer matrix. 21,22he PS matrix served as a heterogeneous interface for controlling the morphology and composition of bicomponent nanocrystals synthesized by a seed-mediated method: AgNCs as seeds partially embedded in the PS matrix as templates to generate the bi-component nanocrystals.The as-made silverbased bicomponent nanocrystals xed in a polystyrene matrix can be used to eliminate the loss of nanocrystals during the washing process.The reusability of Ag-based nanocrystals as catalysts for 4-NP reduction can be characterized by the catalytic performance of 4-NP reduction in multi-cycle reactions.The catalytic performance can be characterized by the variation of 4-NP concentration (absorption peak at 400 nm) with reaction time.For ower-like Au-AgNC nanocrystals freely suspended in the reaction solution, the rate of change of 4-NP concentration with the reaction time decreased signicantly with the increase of the number of reaction cycles (as shown in Fig. 2(A)).This can be attributed to the decrease in the amount of ower-like Au-AgNC nanocrystals in the reaction solution during the washing process, as shown in the extinction spectra of ower-like Au-AgNC nanocrystals in one to three reaction cycles in Fig. 2(B).This result indicated that the reusability of freely dispersed nanocrystals as catalysts was poor.However, the reusability of nanocrystals as catalysts can be efficiently enhanced by xed ower-like Au-AgNCs in a polystyrene matrix, as shown by the changes in the 4-NP concentration in the multi-cycle test in Fig. 2(D).The extinction spectra of ower-like Au-AgNC nanocrystals in a polystyrene matrix showed that the number of nanocrystals remained unchanged during the multi-cycle test as shown in Fig. 2(E).The concentration of 4-NP (relative intensity of the absorption peak at 400 nm, I/I 0 ) had an exponential decay relationship with the reaction time, indicating that the kinetic mechanism of using freely suspended nanocrystals and xed nanocrystals as catalysts for the 4-NP reduction was the rst-order reaction as shown in Fig. 2 (C), (F), and ESI Table S1.† And the reaction rate (reaction constant, K) of 4-NP reduction in both cases also conrmed that the reusability of xed nanocrystals as catalysts was higher than that of freely dispersed nanocrystals as catalysts.

The amount of catalyst used
The other important factor for changes in the reaction rate of 4-NP reduction was the concentration of catalysts in the reaction solution.To compare the concentrations of freely dispersed Au-Ag nanocrystals and xed Au-Ag nanocrystals for 4-NP reduction catalysts, the concentration of Au-AgNCs was calculated from the number of 1 cm × l cm substrates.Aer the release of Au-AgNC nanocrystals from the polystyrene matrix, the plasmon resonance intensity in the extinction spectrum of freely dispersed Au-AgNC nanocrystals can be used to quantify the amount relative to the 1 cm × l cm substrate with xed Au-AgNC nanocrystals.For different concentrations of ower-like Au-AgNC nanocrystals as 4-NP reduction catalysts, the change of 4-NP (I/I 0 ) concentration with reaction time was accelerated with the increase of catalyst concentration in the reaction solution as shown in ESI S1 † and Fig. 3(A).And the kinetic mechanism of 4-NP reduction maintained a rst-order reaction with the change of catalyst concentration, I/I 0 decaying exponentially with reaction time, as shown in ESI Table S2.† The concentration of freely dispersed ower-like nanocrystals as the 4-NP reduction catalysts exhibited a linear relationship with reduction rate, as shown in Fig. 3(B).Similar catalytic performance, linear reduction rate with catalyst concentration, and kinetic reaction mechanism, rst-order reaction, can be observed in xed ower-like Au-AgNC nanocrystals as 4-NP reduction catalysts, as shown in Fig. 3(C), (D), and ESI S2 and Table S3.† However, freely dispersed nanocrystals as catalysts showed higher reduction reactivity than xed nanocrystals as catalysts.This result was because the overall reaction surface area (# of activation sites) of freely dispersed nanocrystals for 4-NP reduction was higher than that of xed nanocrystals for 4-NP reduction.For freely dispersed ower-like nanocrystals as the 4-NP reduction catalysts, the 4-NP reduction did not start immediately, and the delay time increased with the decrease of freely dispersed ower-like nanocrystal concentration (as shown in Fig. 3(A)).The delay in the reduction of 4-NP can be attributed to the adsorption of water molecules on the catalyst surface, resulting in the need to replace the water molecules on the catalyst surface with 4-NP and NaBH 4 for 4-NP reduction. 23nd the decreases in the catalyst concentration led to an increase in the time required for diffusion of 4-NP and NaBH 4 to reach the catalyst surface, resulting in a further delay of the 4-NP reduction. 24However, for xed Au-Ag nanocrystals for 4-NP reduction catalysts, the 4-NP reduction occurred immediately aer NaBH 4 injection, which resulted from the xed Au-Ag nanocrystals being stored in the air, resulting in no adsorption of water molecules on the catalyst surface for 4-NP reduction.
2.3 Shape of bicomponent nanocrystals: ower-like Au-Ag nanocrystal (higher surface area/ volume ratio) or cage-like Au-Ag nanocrystal (stronger synergistic effect) Another parameter that affected the catalytic performance of Au-AgNC nanocrystals as 4-NP reduction catalysts was the morphology of nanocrystals.Here, the ower-like Au-AgNC nanocrystals and cage-like Au-AgNC nanocrystals were used as 4-NP reduction catalysts to study the shape-dependent catalytic performance of nanocrystals.The concentration of the two different morphologies of Au-AgNC nanocrystals can be characterized by measuring the intensity of the extinction spectrum of the AgNC array on a polystyrene matrix, which was used to synthesize Au-AgNC nanocrystals.The concentration of the

Paper Nanoscale Advances
AgNC array in the 1 cm × l cm substrate used for the synthesis of ower-like Au-AgNC nanocrystals (black curve of the extinction spectrum in Fig. 4(A)) was similar to that for the synthesis of cage-like Au-AgNC nanocrystals (red curve of the extinction spectrum in Fig. 4(B)), the concentration of ower-like Au-AgNC nanocrystals in the substrate can be considered to be the same as that of cage-like Au-AgNC nanocrystals.The reduction rate of 4-NP with two ower-like Au-AgNC substrates as catalysts (red circle dot in Fig. 4(C) and ESI S4 †) was higher than that of two cage-like Au-AgNC substrates as catalysts (black square dot in Fig. 4(C) and ESI S4 †).This result was caused by the fact that ower-like Au-AgNC nanocrystals had more activation sites (huge surface area/volume ratio) than cage-like Au-AgNC nanocrystals.Even though the surface area of cage-like Au-AgNC nanocrystals was smaller than that of pristine AgNCs (as theoretical calculation in supporting information S6 †), the reduction rate of 4-NP with two cage-like Au-AgNC substrates as catalysts was similar to that of two pristine AgNC substrates (blue triangle dot in Fig. 4(C) and ESI S4 †).This can be attributed to the abundant Au-Ag alloy in the cage-like nanocrystal, which led to the enhanced "synergetic effect "created between Au and Ag atoms.This strong "synergetic effect "can result in an increase in the reactivity of 4-NP reduction, as shown in ESI S5(B).† The kinetic mechanism of using xed cage-like Au-AgNC nanocrystals as catalysts for the 4-NP reduction reaction also exhibited rst-order reaction (the 4-NP concentration decayed exponentially with reaction time) over a wide range of nanocrystal concentrations as shown in Fig. 4(B) and ESI S3 and Table S4.† However, the reduction rate (reaction constant, K) of As the concentration of cage-like Au-AgNCs increases, the 4-NP reduction preferentially occurred on the Au-Ag alloy frame, which led to a signicant increase in 4-NP reduction reactivity (exponential increasing) due to the "synergetic effect" between Au and Ag atoms.This deviation should be attributed to the stronger "synergetic effect" between Au and Ag atoms for 4-NP reduction in cage-like Au-AgNC nanocrystals than in ower-like Au-AgNC nanocrystals (the atomic content of Au in cage-like Au-AgNC nanocrystals was 8.8 times higher than in ower-like Au-Ag nanocrystals, as shown in ESI S5 †).And with the increase in cage-like Au-AgNC concentration (# of the substrate), the "synergetic effect" of 4-NP reduction was inten-sied, resulting in a rapid increase in the 4-NP reduction rate.

Component of bicomponent nanocrystals: Au-Ag nanocrystal or Ag 2 S-Ag nanocrystals
Besides noble metals that can be used as 4-NP reduction catalysts, Ag 2 S had also been demonstrated to be an excellent 4-NP reduction catalyst. 14,15Here, Ag 2 S-AgNC nanocrystals were synthesized by a suldation reaction on the AgNC surface. 22The core-shell Ag 2 S-AgNC nanocrystals were used as 4-NP reduction catalysts and the catalytic performance was compared with that of Au-AgNC nanocrystals.The concentration of core-shell Ag 2 S-AgNC nanocrystals can also be characterized by measuring the intensity of the extinction spectrum of the AgNC array on a polystyrene matrix for the synthesis of core-shell Ag 2 S-AgNC nanocrystals (as shown in the red curve in Fig. 5(A)), and the concentration needed to be adjusted by comparing the intensity of the extinction spectrum of the AgNC array on a polystyrene matrix for the synthesis of ower-like Ag-AgNC nanocrystals (as shown in the black curve in Fig. 5(A)).The result showed that the concentration of core-shell Ag 2 S-AgNC nanocrystals (# of Ag 2 S-AgNC) on one substrate was close to 0.88 times that of ower-like Au-AgNC nanocrystals on one substrate.Therefore, the adjusted Ag 2 S-AgNC nanocrystal concentration (# of the substrate) for 4-NP reduction was equal to 0.88 times the actual number of substrates used for 4-NP reduction.The kinetic mechanism of Ag 2 S-AgNC nanocrystals as 4-NP reduction catalysts was also the rst-order reaction over a wide range of nanocrystal concentrations as shown in Fig. 5(B) and ESI S6 and Table S5.† However, the reduction rate (reaction constant, K) of 4-NP showed an exponential growth and saturation relationship with the catalyst concentration.And the reduction rate of 4-NP with core-shell Ag 2 S-AgNC nanocrystals as catalysts was much lower than that with ower-like Au-AgNC nanocrystals as catalysts (red circle dot in Fig.

Nanoscale Advances
Paper reduction catalysts should be effectively enhanced under irradiation excitation, which resulted from the generation of hot electrons around Ag-based nanocrystals.Here, the hot electrons were generated by ower-like Au-AgNC nanocrystals at an irradiation wavelength of 520 nm (corresponding to the plasmonic mode of ower-like Au-AgNC nanocrystals shown in Fig. 6(A)) and used to reduce 4-NP.Compared with the owerlike Au-Ag nanocrystals without irradiation assistance (without hot electrons), the ower-like Au-Ag nanocrystals with irradiation assistance have a faster reaction rate of 4-NP reduction, as shown in Fig. 6(B).And the enhancement factor (reaction rate (k) with irradiation assistance/reaction rate without irradiation assistance) increased with the number of ower-like Au-Ag nanocrystals as shown in Fig. 6(C) and ESI Table S7.† This phenomenon is due to the increase in the number of hot electrons for enhancing the reduction reaction of 4-NP with the increase of catalyst concentration under the same irradiation power.
Here, Ag-based nanocrystals were used as catalysts for the 4-NP reduction reaction.The reusability of the catalyst can be improved by xing the catalyst in the polymer matrix.The catalytic performance of these Ag-based nanocrystals strongly depended on their morphologies and components, which are caused by the surface area/volume and synergistic effects, respectively.Since the catalytic activity strongly depended on the amount of catalyst and the concentration-reducing agent (NaBH 4 ) and inconsistencies in the use of these parameters for catalytic activity studies in previous reports, it is difficult to demonstrate the catalytic performance directly using the reaction rate (reaction time).Here, the ratio of the amount of catalyst to the amount of 4-NP in aqueous solution and the reaction completion time was used to represent the catalytic performance and comparison with different literature studies, as shown in the ESI Tables S8 and S12.† The catalytic performance of the ower-like Au-Ag nanocrystals indicated that a smaller amount of nanocrystals can be used to degrade the same concentration of 4-NP within the same reaction time period than catalysts in the literature.
These Ag-based nanocrystals with special morphology and composition on a PS matrix used as 4-NP reduction catalysts showed higher catalytic performance (at least two orders of magnitude fewer nanocrystal numbers than in the literature can be used to treat the same concentration of 4-NP in aqueous solution, as shown in ESI S11 †). 25 The catalytic performance of Ag-based nanocrystals can be further enhanced by generating hot electrons around the nanocrystals under irradiation.These results pave the way for designing excellent catalysts with multiple enhancement effects, such as surface area/volume, synergistic effect, and hot electron assisted effect.

Conclusions
Silver-based nanocrystals have excellent catalytic performance in various reactions, such as 4-PN reduction.Here, bimetallic nanocrystals (Au-Ag) and metal-semiconductor (Ag-Ag 2 S) nanocrystals with highly heterogeneous morphologies, which can be fabricated by a seed-mediated method in the heterogeneous interface (polymer lm), act as catalysts for the reduction of 4-NP.Since the heterogeneous nanocrystals are xed in the polymer lm, the reusability of the catalysts is signicantly improved compared to the catalysts that are freely dispersed in the reaction solution.These heterogeneous nanocrystals have different morphologies and compositions, leading to different surface area/volume ratios and synergistic effects, resulting in different catalytic performances.The ower-like Au-Ag nanocrystals with higher surface area/volume ratio and cage-like Au-Ag nanocrystals with stronger synergistic effects show faster 4-NP reduction than pristine Ag nanocrystals.And the reduction of Ag 2 S to Ag atom is a competitive reaction with the reduction of 4-NP, resulting in a slower reaction rate of Ag 2 S-Ag nanocrystals than pristine Ag nanocrystals.The catalytic performance of Ag-based nanocrystals can be further enhanced by generating hot electrons around nanocrystals under irradiation.These results show that by carefully controlling the morphology and composition of nanocrystals, it is possible to design and fabricate excellent catalysts for various reactions.

Synthesis of shaped AgNCs
AgNCs were synthesized by using the polyol synthetic method which has been reported in previous literature.The AgNO 3 precursor solution was prepared by dissolving 0.20 g of AgNO 3 in 5 mL of 1,5-pentanediol with 44 mL of 0.043 M CuCl 2 solution.Another precursor solution was prepared by dissolving 0.10 g of PVP in 5 mL of 1,5-pentanediol.The reaction solution was prepared by heating 10 mL of 1,5-pentanediol in a 50 mL glass round-bottom ask with continuous stirring in an oil bath heated to 193 °C.AgNO 3 and PVP precursor solutions were injected alternately into the hot reaction solution at rates of 500 mL of AgNO 3 precursor solutions per min and 320 mL of PVP precursor solutions per 30 s.Some reaction parameters, such as the total volume of precursor injection in the reaction batch and reaction temperature, can be used to control the size of AgNCs.To obtain highly uniform heterogeneous nanocrystals through the seed-mediated synthesis method, the quality (shape and size) of AgNCs (seeds) needs to be enhanced, which can be achieved by a post-synthetic purication process.The as-made AgNC colloidal solution contained ∼20% impurities of other shapes, such as triangular, spherical, and wire-like nanocrystals, and the uniformity of AgNCs could be increased to

Paper
Nanoscale Advances >95% aer four times of ltration with 450 nm lter paper and six times with 220 nm lter paper.

Deposition of polystyrene thin lms on the substrate
There are three steps for the deposition of PS lms on silicon/ glass substrates: (1) clean silicon/glass substrates with a freshly prepared piranha solution (70% (v) concentrated H 2 SO 4 and 30% (v) H 2 O 2 ); (2) formation of a hydrophobic coating on the substrate by treated substrates with hexamethyldisilazane (HMDS) vapor, which can be used to enhance the adhesion force between the substrate and the polymer thin lm; (3) deposition of the PS lm on substrates; PS (M w = 35 000) was dissolved in a toluene solution (5.8 wt%) for deposition of thin lms on the substrate via the spin-coating process.The thickness of PS lms on substrates can be controlled by the concentration of PS solution and spin speed.

Deposition of AgNC arrays on PS lms
To obtain AgNC arrays on PS lms, the as-synthesized and puri-ed AgNC colloidal solutions were precipitated in ethanol and then dispersed in CHCl 3 .Then, the colloidal solution of AgNCs/ CHCl 3 was added dropwise to the water-air interface of a glass Petri dish with water, and CHCl 3 leaving volatilized to leave a monolayer of silver nanocrystals with isotopically distributed oating on the water-air interface.The surface tension of the AgNC monolayer array at the water-air interface can be used to control the concentration (surface coverage) of the AgNC array.The AgNC monolayer array was then transferred onto the PS lms by dip-coating.The AgNC array on the PS lm can then be embedded into the PS lm by thermal treatment at a temperature above the glass-transition temperature of PS (T > T g of PS ).The embedding depth of AgNCs in the PS lm can be controlled by thermal treatment conditions (treatment temperature and time).The color of the aqueous solution immediately changed from colorless to yellow (nitrophenolate ions).The external light source is an LED point light source with a wavelength of ∼520 nm and power ∼9.9 W which was used to generate the "hot electrons" on nanocrystals.The spot size of the external light source on the nanocomposite sample is about 1 cm in diameter (sample size 1 cm × 1 cm square), which can be adjusted by changing the distance between the light source and the sample.The power density of irradiation is ∼12.6 W cm −2 .Then, the variation of the absorption peak intensity of nitrophenolate ions (∼400 nm) with reaction time was used to observe the reduction rate of 4-NP.

Fig. 1 Fig. 2
Fig.1Schematic of silver-based heterogeneous nanocrystals as catalysts for the reduction of 4-nitrophenol (4-NP).There are various catalytic results that characterized the catalytic performance of catalysts: reusability, concentration-dependent, shape-dependent, synergetic effects, composition-dependent, and the plasmon enhancement effect (photocatalyst).

Fig. 3
Fig. 3 Changes in the reactivity of 4-NP reduction with different concentrations of flower-like Au-AgNC nanocrystals as catalysts.(A) For the nanocrystals freely suspended in the reaction solution, the concentration of 4-NP varied with reaction time at different nanocrystal concentrations.The dashed line was generated by fitting the curve with an exponential equation:I ¼ I 0 þ A Â exp Àðt À t 0 Þ B ,here I: the concentration of 4-NP, I 0 : the concentration of 4-NP at the start of the reaction and 1/B: reaction constant (k).(B) The rate of the 4-NP reduction reaction (reaction constant) varied with the concentration of Au-AgNCs (C, corresponding to the # of substrates, Au-AgNC array in a polymer matrix, releasing in the solution).The relationship between k and C was linear.(C) For the nanocrystals fixed in a polymer matrix, the concentration of 4-NP varied with reaction time at different nanocrystal concentrations.The dashed line was generated by fitting the curve with an exponential equation.(D) the rate of the 4-NP reduction reaction (reaction constant) varied with the concentration of Au-AgNCs (C, # of substrates, Au-AgNC array in a polymer matrix).The relationship between k and C was linear.
5(C)), which may be attributed to the reduction of Ag + ions in Ag 2 S to Ag atoms assisted by Ag and NaBH 4 .The reduction of Ag + ions in Ag 2 S to Ag atoms was a competitive reaction with the reduction of 4-NP, which led to a decrease in the reduction rate of 4-NP.The coreshell Ag 2 S-AgNC nanocrystals underwent the shape change during the 4-NP reduction (as shown in the SEM image in ESI S8(A) †), which can be used as evidence for the reduction of Ag + ions in Ag 2 S to Ag atoms.And the rounded core-shell Ag 2 S-AgNC nanocrystals as 4-NP reduction catalysts showed a faster 4-NP reduction rate than core-shell Ag 2 S-AgNC nanocrystals as

Fig. 4
Fig. 4 Changes in the reactivity of 4-NP reduction with different concentrations of cage-like Au-AgNC nanocrystals as catalysts.(A) Extinction spectra of the AgNC array in a polystyrene matrix, which were used to fabricate flower-like Au-AgNC (black curve) and cage-like Au-AgNC (red curve).SEM image of cage-like Au-Ag nanocrystals as an inset image.(B) The concentration of 4-NP varied with reaction time at different nanocrystal concentrations.The dashed line was generated by fitting the curve with an exponential equation.(C) the rate of the 4-NP reduction reaction (reaction constant) varied with the concentration of Au-AgNCs (C, # of substrates, Au-AgNC array in a polymer matrix).k exhibited an exponential growth relationship with the increase of C. The reaction rate of 4-NP reduction was compared between pristine AgNCs (blue triangle) and flower-like Au-AgNC nanocrystals (red circle).The scale bar was 100 nm.

Fig. 5
Fig. 5 Changes in the reactivity of 4-NP reduction with different concentrations of Ag 2 S-AgNC nanocrystals as catalysts.(A) Extinction spectra of the AgNC array in a polystyrene matrix, which was used to fabricate flower-like Au-AgNCs (black curve) and Ag 2 S-AgNCs (red curve).SEM image of cage-like Au-Ag nanocrystals as an inset image.(B)The concentration of 4-NP varied with reaction time at different nanocrystal concentrations.The dashed line was generated by fitting the curve with an exponential equation.(C) the rate of the 4-NP reduction reaction (reaction constant) varied with the concentration of Au-AgNCs (C, # of substrates, Au-AgNC array in a polymer matrix).k exhibited an exponential saturation relationship with the increase of C. The reaction rate of 4-NP reduction was compared with flower-like Au-AgNCs (blue triangle) and cage-like Au-AgNC nanocrystals (red circle).The scale bar was 100 nm.

4. 8
Catalytic performance test of silver-based nanocrystals xed on a PS matrix as catalysts for the reduction of 4nitrophenolThe as-made Ag-based nanocrystals on the PS matrix were mounted on a plastic plate (as shown in the schematic in ESI S10 †) and placed in a quartz cuvette.1.7 mM 4-NP aqueous solution (2.087 mg 4-NP dissolved in 8.82 ml DI water) and 0.4 M NaBH 4 aqueous solution (38 mg NaBH 4 dissolved in 2.5 ml DI water) were prepared for 4-NP reduction test.For the 4-NP reduction test, 2.5 ml DI water and 150 ml 1.7 mM 4-NP aqueous solution were added to a quartz cuvette with an Ag-based nanocrystal-PS matrix.And then 150 ml 0.4 M NaBH 4 aqueous solution was injected into the quartz cuvette (reaction time = 0 min).The color of the aqueous solution immediately changed from colorless to yellow (nitrophenolate ions).Then, the variation of the absorption peak intensity of nitrophenolate ions (∼400 nm) with reaction time was used to observe the reduction rate of 4-NP.Nanoscale Advances Paper 4.9 Catalytic performance test of freely dispersed silverbased nanocrystals as catalysts for the reduction of 4nitrophenol The as-made Ag-based nanocrystals on the PS matrix were placed in chloroform to remove Ag-based nanocrystals from the PS matrix.And Ag-based nanocrystals were then dispersed in DI water.1.7 mM 4-NP aqueous solution (2.087 mg 4-NP dissolved in 8.82 ml DI water) and 0.4 M NaBH 4 aqueous solution (38 mg NaBH 4 dissolved in 2.5 ml DI water) were prepared for the 4-NP reduction test.For the 4-NP reduction test, 2.6 ml DI water and 150 ml 1.7 mM 4-NP aqueous solution were added to a quartz cuvette with free dispersed Ag-based nanocrystals.And then 150 ml of 0.4 mM NaBH 4 aqueous solution was injected into the quartz cuvette (reaction time = 0 min).The color of the aqueous solution immediately changed from colorless to yellow (nitrophenolate ions).Then, the variation of the absorption peak intensity of nitrophenolate ions (∼400 nm) with reaction time was used to observe the reduction rate of 4-NP.4.10 Catalytic performance test of ower-like Au-AgNC nanocrystals xed on a PS matrix as photocatalysts for the reduction of 4-nitrophenol The as-made ower-like Au-AgNC nanocrystals on the PS matrix were mounted on a plastic plate (as shown in the schematic in ESI S10 †) and placed in a quartz cuvette.1.7 mM 4-NP aqueous solution (2.087 mg 4-NP dissolved in 8.82 ml DI water) and 0.4 M NaBH 4 aqueous solution (38 mg NaBH 4 dissolved in 2.5 ml DI water) were prepared for 4-NP reduction test.For the 4-NP reduction test, 2.5 ml DI water and 150 ml 1.7 mM 4-NP aqueous solution were added to a quartz cuvette with an Ag-based nanocrystal-PS matrix.And then 150 ml of 0.4 M NaBH 4 aqueous solution was injected into the quartz cuvette (reaction time = 0 min).
AgNCs partially embedded in the polymer matrix as a template to synthesize ower-like Au-AgNC nanocrystals This AgNC-PS-glass or silicon substrate was hung in an aqueous solution for the synthesis of bicomponent nanocrystals.Dissolving 1 mg of PVP in a 20 ml glass vial with 12 ml of DI water (0.0015 mM) gave the reaction solution.Under magnetic stirring, 11.2 ml of 1 mM HAuCl 4 solution was injected into the reaction solution every 20 minutes, and Au-Ag bimetallic nanocrystals were formed by reducing Au 3+ ions.The change of optical properties with reaction time can be characterized by measuring the extinction spectrum of the AgNC-PS-glass substrate.And the shape change of Au-Ag alloy nanocrystals with time can be observed by SEM and HRTEM. 214.7 Using AgNCs partially embedded in the polymer matrix as a template to synthesize core-shell-like Ag 2 S-Ag nanocrystals.The AgNC was partially embedded into the PS lm by thermal treatment, and its embedding depth (H) was about H ∼ L/3 by (L is the length of AgNCs) (as ESI S1 †).This AgNC-PS-glass or silicon substrate was hung in an aqueous solution for the synthesis of bicomponent nanocrystals.Dissolving 12 mg of PVP in a 20 ml glass vial with 18 ml of DI water (0.018 mM) as a reaction solution.Two reaction precursor solutions were prepared by dissolving 16.4 mg of S powder and 72.2 mg of Na 2 S-9H 2 O in 6.3 ml of DI water at 80 °C with magnetic stirring for 12 h (forming the 0.047 mM Na 2 S x solution).The color of the Na 2 S x aqueous solution is bright yellow.And dilute the Na 2 S x aqueous solution to 0.0004 mM (10 mL of 0.047 mM Na 2 S x aqueous solution + 1.2 mL DI H 2 O).Under magnetic stirring, 10 ml of 0.0004 mM Na 2 S x solution was injected into the reaction solution every 20 minutes, and Ag 2 S-Ag bicomponent nanocrystals were formed.The change of optical properties with reaction time can be characterized by measuring the extinction spectrum of the AgNC-PS-glass substrate.And the shape change of Au-Ag alloy nanocrystals with time can be observed by SEM and HRTEM.
214.6 Using AgNCs partially embedded in the polymer matrix as a template to synthesize cage-like Au-AgNC nanocrystalsThe AgNC was partially embedded into the PS lm by thermal treatment, and its embedding depth (H) was about H ∼ 2L/3 (L is the length of AgNCs).